Table 19. Continued. 













Corrosion 







Alloy 



CDA 



No." 



Environment 



Exposure 

 (day) 



Depth 



(ft) 



Rate 



(mpy) 



Type of 

 Corrosion c 



Source 



Al Bronze, 10% 



_ 



W 



402 



2,370 



0.3 



S-DA 



INCO (3) 



Al Bronze, 10% 



- 



S 



402 



2,370 



<0.1 



MO-DA 



INCO (3) 



Al Bronze, 10% 



- 



W 



181 



5 



2.1 



MO-DA 



INCO (3) 



Al Bronze, 10% 



- 



W 



366 



5 



1.3 



MO-DA 



INCO (3) 



Al Bronze, 11%* 



- 



W 



123 



5,640 



0.4 



U 



MEL (5) 



Al Bronze, 11% 



- 



w 



123 



5,640 



0.5 



V-SL-DA 



INCO (3) 



Al Bronze, 11% 



- 



s 



123 



5,640 



0.4 



V-SL-DA 



INCO (3) 



Al Bronze, 11% 



- 



w 



403 



6,780 



0.1 



SL-DA 



INCO (3) 



Al Bronze, 11% 



- 



s 



403 



6,780 



<0.1 



SL-DA 



INCO (3) 



Al Bronze, 1 1% 



- 



w 



751 



5,640 



0.8 



SL-DA 



INCO (3) 



Al Bronze, 11% 



- 



w 



751 



5,640 



0.3 



U-P 



MEL (5) 



Al Bronze, 11% 



- 



s 



751 



5,640 



0.1 



V-SL-DA 



INCO (3) 



Al Bronze, 11% 



- 



w 



1,064 



5,300 



0.1 



SL-DA 



INCO (3) 



Al Bronze, 11% 



- 



s 



1,064 



5,300 



0.2 



MO-DA 



INCO (3) 



Al Bronze, 11% 



- 



w 



197 



2,340 



0.2 



SL-DA g 

 SL-DA* 



INCO (3) 



Al Bronze, 11% 



- 



s 



197 



2,340 



<0.1 



INCO (3) 



Al Bronze, 11% 



- 



w 



402 



2,370 



0.2 



MO-DA 



INCO (3) 



Al Bronze, 11% 



- 



s 



402 



2,370 



<0.1 



SL-DA 



INCO (3) 



Al Bronze, 11% 



- 



w 



366 



5 



1.1 



U 



INCO (3) 



Al Bronze, 13% e 



- 



w 



123 



5,640 



0.5 



V-SL-DA 



INCO (3) 



Al Bronze, 13% 



- 



s 



123 



5,640 



0.5 



V-SL-DA 



INCO (3) 



Al Bronze, 13% 



- 



w 



403 



6,780 



0.6 



S-DA 



INCO (3) 



Al Bronze, 13% 



- 



s 



403 



6,780 



<0.1 



SL-DA 



INCO (3) 



Al Bronze, 1 3% 



- 



w 



751 



5,640 



1.9 



S-DA 



INCO (3) 



Al Bronze, 13% 



- 



s 



751 



5,640 



0.5 



MO-DA 



INCO (3) 



Al Bronze, 1 3% 



- 



w 



1,064 



5,300 



0.6 



S-DA 



INCO (3) 



Al Bronze, 1 3% 



- 



s 



1,064 



5,300 



0.3 



SL-DA 



INCO (3) 



Al Bronze, 1 3% 



- 



w 



197 



2,340 



0.4 



MO-DA 



INCO (3) 



Al Bronze, 13% 



- 



s 



197 



2,340 



<0.1 



SL-DA 



INCO (3) 



Al Bronze, 13% 



- 



w 



402 



2,370 



0.3 



MO-DA 



INCO (3) 



Al Bronze, 1 3% 



- 



s 



402 



2,370 



<0.1 



SL-DA 



INCO (3) 



Al Bronze, 1 3% 



- 



w 



181 



5 



2.1 



S-DA 



INCO (3) 



Al Bronze, 1 3% 



- 



w 



366 



5 



1.9 



S-DA 



INCO (3) 



Ni-Al Bronze 



- 



w 



123 



5,640 



0.6 



P 



MEL (5) 



Ni-Al Bronze 



- 



w 



751 



5,640 



0.4 



P(21) 



MEL (5) 



Ni-Al Bronze No. 1 



- 



w 



123 



5,640 



0.5 



U 



MEL (5) 



Ni-Al Bronze No. 1 



- 



w 



123 



5,640 



0.4 



I-P 



INCO (3) 



Ni-Al Bronze No. 1 



- 



s 



123 



5,640 



0.2 



I-P 



INCO (3) 



Ni-Al Bronze No. 1 



- 



w 



403 



6,780 



0.3 



I-P 



INCO (3) 



Ni-Al Bronze No. 1 



- 



s 



403 



6,780 



0.1 



U 



INCO (3) 



Ni-Al Bronze No. 1 



- 



w 



751 



5,640 



1.1 



C(16);P 



INCO (3) 



Ni-Al Bronze No. 1 



- 



w 



751 



5,640 



0.2 



P 



MEL (5) 



Ni-Al Bronze No. 1 



- 



s 



751 



5,640 



0.3 



P(17) 



INCO (3) 



Ni-Al Bronze No. 1 



- 



w 



1,064 



5,300 



0.1 



P(8) 



INCO (3) 



Ni-Al Bronze No. 1 



- 



s 



1,064 



5,300 



1.2 



CR(30) 



INCO (3) 



Ni-Al Bronze No. 1 



- 



w 



197 



2,340 



0.3 



U 



INCO (3) 



Ni-Al Bronze No. 1 





s 



197 



2,340 



<0.1 



U-ET 



INCO (3) 



74 



